 
data_fr12 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H2 Ca Fe3 K0.50 Mg5 Na0.50 O24 Si5' 
_chemical_formula_weight          886.69 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ca'  'Ca'   0.2262   0.3064 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mg'  'Mg'   0.0486   0.0363 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Si'  'Si'   0.0817   0.0704 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            ? 
_symmetry_space_group_name_H-M    ? 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, y, -z' 
 'x+1/2, y+1/2, z' 
 '-x+1/2, y+1/2, -z' 
 '-x, -y, -z' 
 'x, -y, z' 
 '-x+1/2, -y+1/2, -z' 
 'x+1/2, -y+1/2, z' 
 
_cell_length_a                    9.8165(2) 
_cell_length_b                    18.0126(5) 
_cell_length_c                    5.3002(14) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  105.380(4) 
_cell_angle_gamma                 90.00 
_cell_volume                      903.6(2) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     ? 
_cell_measurement_theta_min       ? 
_cell_measurement_theta_max       ? 
 
_exptl_crystal_description        ? 
_exptl_crystal_colour             ? 
_exptl_crystal_size_max           ? 
_exptl_crystal_size_mid           ? 
_exptl_crystal_size_min           ? 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.259 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              874 
_exptl_absorpt_coefficient_mu     3.430 
_exptl_absorpt_correction_type    ? 
_exptl_absorpt_correction_T_min   ? 
_exptl_absorpt_correction_T_max   ? 
_exptl_absorpt_process_details    ? 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   ? 
_diffrn_measurement_method        ? 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             13231 
_diffrn_reflns_av_R_equivalents   0.0462 
_diffrn_reflns_av_sigmaI/netI     0.0398 
_diffrn_reflns_limit_h_min        -17 
_diffrn_reflns_limit_h_max        17 
_diffrn_reflns_limit_k_min        -32 
_diffrn_reflns_limit_k_max        32 
_diffrn_reflns_limit_l_min        -9 
_diffrn_reflns_limit_l_max        9 
_diffrn_reflns_theta_min          3.99 
_diffrn_reflns_theta_max          40.71 
_reflns_number_total              2840 
_reflns_number_gt                 2071 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0297P)²+0.5658P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.0069(4) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          2840 
_refine_ls_number_parameters      116 
_refine_ls_number_restraints      3 
_refine_ls_R_factor_all           0.0548 
_refine_ls_R_factor_gt            0.0308 
_refine_ls_wR_factor_ref          0.0694 
_refine_ls_wR_factor_gt           0.0621 
_refine_ls_goodness_of_fit_ref    0.946 
_refine_ls_restrained_S_all       0.946 
_refine_ls_shift/su_max           0.752 
_refine_ls_shift/su_mean          0.200 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
T1 Si 0.28484(4) 0.085290(19) 0.30361(8) 0.00866(8) Uani 1 1 d . . . 
T2 Si 0.29145(4) 0.172670(18) 0.81034(7) 0.00688(7) Uani 1 1 d . . . 
M1 Mg 0.0000 0.07962(2) 0.5000 0.01026(10) Uani 0.501(3) 2 d SP . . 
M11 Fe 0.0000 0.07962(2) 0.5000 0.01026(10) Uani 0.499(3) 2 d SP . . 
M2 Mg 0.0000 0.17705(2) 0.0000 0.00693(13) Uani 0.800(3) 2 d SP . . 
M22 Fe 0.0000 0.17705(2) 0.0000 0.00693(13) Uani 0.200(3) 2 d SP . . 
M3 Mg 0.0000 0.0000 0.0000 0.00730(14) Uani 0.682(3) 4 d SP . . 
M33 Fe 0.0000 0.0000 0.0000 0.00730(14) Uani 0.318(3) 4 d SP . . 
M4 Ca 0.0000 0.27860(6) 0.5000 0.01021(16) Uani 0.892(7) 2 d SP . . 
M42 Mg 0.0000 0.2573(11) 0.5000 0.016(3) Uiso 0.107(10) 2 d SP . . 
A1 Na 0.5282(7) 0.0000 0.0586(11) 0.055(3) Uani 0.529(10) 2 d SP . . 
A2 K 0.0000 0.4659(15) 0.0000 0.039(5) Uiso 0.050(6) 2 d SP . . 
O1 O 0.10776(10) 0.08648(5) 0.2195(2) 0.00929(15) Uani 1 1 d . . . 
O2 O 0.11798(10) 0.17048(5) 0.7265(2) 0.00958(15) Uani 1 1 d . . . 
O3 O 0.10423(15) 0.0000 0.7154(3) 0.0127(2) Uani 1 2 d S . . 
O4 O 0.36431(11) 0.25155(5) 0.7885(2) 0.01262(17) Uani 1 1 d . . . 
O5 O 0.35135(11) 0.14023(6) 0.1090(2) 0.01303(17) Uani 1 1 d . . . 
O6 O 0.34857(11) 0.11834(6) 0.6079(2) 0.01341(17) Uani 1 1 d . . . 
O7 O 0.34548(17) 0.0000 0.2841(4) 0.0175(3) Uani 1 2 d S . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
T1 O7 1.6607(7) . ? 
T1 O1 1.6762(10) . ? 
T1 O6 1.6768(12) . ? 
T1 O5 1.6813(10) . ? 
T1 A2 3.115(8) 7 ? 
T1 M3 3.2220(4) . ? 
T1 M4 3.2233(9) 7_556 ? 
T1 M1 3.2336(4) . ? 
T1 O4 3.2620(10) 7_556 ? 
T1 A1 3.359(5) 5_655 ? 
T1 A1 3.376(5) . ? 
T1 A2 3.671(15) 3_545 ? 
T2 O4 1.6086(10) . ? 
T2 O2 1.6424(10) . ? 
T2 O5 1.6430(11) 1_556 ? 
T2 O6 1.6560(10) . ? 
T2 M4 3.0747(5) 7_556 ? 
T2 M42 3.205(8) 7_556 ? 
T2 A2 3.22(2) 7_556 ? 
T2 O4 3.2322(11) 7_557 ? 
T2 O4 3.4206(13) 7_556 ? 
T2 M4 3.4692(7) . ? 
T2 O4 3.7614(12) 2_657 ? 
T2 O7 3.9438(13) 1_556 ? 
M1 O3 1.9460(11) 5_556 ? 
M1 O3 1.9460(11) . ? 
M1 O1 2.0440(9) . ? 
M1 O1 2.0440(9) 2_556 ? 
M1 O2 2.1735(10) . ? 
M1 O2 2.1735(10) 2_556 ? 
M1 M11 2.8683(8) 5_556 ? 
M1 M1 2.8683(8) 5_556 ? 
M1 M3 3.0133(6) . ? 
M1 M33 3.0133(6) 1_556 ? 
M1 M3 3.0133(6) 1_556 ? 
M2 O4 1.9731(11) 7_556 ? 
M2 O4 1.9731(11) 8_454 ? 
M2 O2 2.0849(9) 2_556 ? 
M2 O2 2.0849(9) 1_554 ? 
M2 O1 2.1170(10) 2 ? 
M2 O1 2.1170(11) . ? 
M2 M42 3.019(10) . ? 
M2 M42 3.019(10) 1_554 ? 
M2 M11 3.1786(7) 1_554 ? 
M2 M1 3.1786(7) 1_554 ? 
M3 O3 2.0352(14) 5_556 ? 
M3 O3 2.0352(14) 1_554 ? 
M3 O1 2.0608(10) 5 ? 
M3 O1 2.0608(10) . ? 
M3 O1 2.0608(10) 6 ? 
M3 O1 2.0608(10) 2 ? 
M3 M11 3.0133(6) 5 ? 
M3 M1 3.0133(6) 5 ? 
M3 M11 3.0133(6) 5_556 ? 
M3 M1 3.0133(6) 5_556 ? 
M4 O4 2.3425(11) 7_556 ? 
M4 O4 2.3425(11) 8_455 ? 
M4 O2 2.4161(13) 2_556 ? 
M4 O2 2.4161(13) . ? 
M4 O6 2.5366(13) 7_556 ? 
M4 O6 2.5366(13) 8_455 ? 
M4 O5 2.6377(13) 7_556 ? 
M4 O5 2.6377(13) 8_455 ? 
M4 T2 3.0747(5) 7_556 ? 
M4 T2 3.0747(5) 8_455 ? 
M42 O2 2.120(15) 2_556 ? 
M42 O2 2.120(15) . ? 
M42 O4 2.2843(18) 8_455 ? 
M42 O4 2.2843(18) 7_556 ? 
M42 M22 3.019(10) 1_556 ? 
M42 M2 3.019(10) 1_556 ? 
M42 T2 3.205(8) 7_556 ? 
M42 T2 3.205(8) 8_455 ? 
A1 A2 0.71(2) 3_545 ? 
A1 A2 0.71(2) 7 ? 
A1 A1 0.714(13) 5_655 ? 
A1 O7 2.405(6) . ? 
A1 O7 2.456(6) 5_655 ? 
A1 O6 2.828(4) 2_656 ? 
A1 O6 2.828(4) 5_656 ? 
A1 T1 3.359(5) 5_655 ? 
A1 T1 3.359(5) 2_655 ? 
A1 O7 3.374(6) 5_656 ? 
A1 T1 3.376(5) 6 ? 
A2 A1 0.71(2) 3_455 ? 
A2 A1 0.71(2) 7 ? 
A2 A2 1.23(5) 5_565 ? 
A2 O7 2.481(7) 3_455 ? 
A2 O7 2.481(7) 7 ? 
A2 O5 2.56(2) 8_455 ? 
A2 O5 2.56(2) 7 ? 
A2 O6 2.682(15) 8_454 ? 
A2 O6 2.682(15) 7_556 ? 
A2 T1 3.115(8) 7 ? 
A2 T1 3.115(8) 8_455 ? 
A2 T2 3.22(2) 8_454 ? 
O1 O7 2.7505(16) . ? 
O1 O4 2.9317(13) 7_556 ? 
O1 O4 4.0678(15) 8_454 ? 
O1 O4 4.4997(15) . ? 
O1 O7 4.8008(19) 5 ? 
O2 M22 2.0849(9) 1_556 ? 
O2 M2 2.0849(9) 1_556 ? 
O2 O4 2.7687(13) . ? 
O2 O4 2.8937(15) 7_557 ? 
O2 O4 2.9521(13) 8_455 ? 
O2 O4 3.1153(15) 7_556 ? 
O2 O7 4.4328(17) 1_556 ? 
O3 M11 1.9460(11) 5_556 ? 
O3 M1 1.9460(11) 5_556 ? 
O3 M33 2.0352(14) 1_556 ? 
O3 M3 2.0352(14) 1_556 ? 
O3 O7 3.303(2) 1_556 ? 
O3 O7 3.702(2) . ? 
O3 O7 4.415(2) 5_556 ? 
O3 O4 5.1195(11) 3_445 ? 
O3 O4 5.1195(11) 8_455 ? 
O3 O4 5.1584(13) 7_557 ? 
O4 M22 1.9731(11) 7_556 ? 
O4 M2 1.9731(11) 7_556 ? 
O4 M42 2.2843(18) 7_556 ? 
O4 M4 2.3425(11) 7_556 ? 
O4 O6 2.5727(14) . ? 
O4 O5 2.6528(14) 1_556 ? 
O4 O2 2.8937(15) 7_557 ? 
O4 O1 2.9317(13) 7_556 ? 
O4 O2 2.9521(13) 8 ? 
O4 O4 2.993(2) 2_657 ? 
O4 O5 3.0310(14) 7_556 ? 
O4 O2 3.1153(15) 7_556 ? 
O4 T2 3.2322(11) 7_557 ? 
O4 T1 3.2620(10) 7_556 ? 
O4 O4 3.279(2) 7_556 ? 
O4 O5 3.3619(14) 2_656 ? 
O4 T2 3.4206(13) 7_556 ? 
O4 O6 3.4561(16) 7_556 ? 
O5 T2 1.6430(11) 1_554 ? 
O5 A2 2.56(2) 7 ? 
O5 M4 2.6377(13) 7_556 ? 
O5 O4 2.6528(14) 1_554 ? 
O5 O7 2.6969(12) . ? 
O5 O4 3.0310(14) 7_556 ? 
O5 O4 3.3619(14) 2_656 ? 
O5 O7 4.5284(19) 5_656 ? 
O5 O7 4.7821(17) 5_655 ? 
O5 O4 5.0235(15) 8_454 ? 
O6 M4 2.5366(13) 7_556 ? 
O6 A2 2.682(15) 7_556 ? 
O6 O7 2.7318(16) . ? 
O6 A1 2.828(4) 5_656 ? 
O6 O4 3.4561(16) 7_556 ? 
O6 O7 3.6028(16) 5_656 ? 
O6 O7 4.177(2) 1_556 ? 
O6 O4 4.3765(16) 2_657 ? 
O6 O4 4.6105(14) 2_656 ? 
O7 T1 1.6607(7) 6 ? 
O7 A1 2.456(6) 5_655 ? 
O7 A2 2.481(7) 7 ? 
O7 A2 2.481(7) 3_545 ? 
O7 O5 2.6969(12) 6 ? 
O7 O6 2.7318(16) 6 ? 
O7 O1 2.7505(16) 6 ? 
O7 O7 3.280(4) 5_656 ? 
O7 O3 3.303(2) 1_554 ? 
O7 A1 3.374(6) 5_656 ? 
O7 O6 3.6028(16) 2_656 ? 
O7 O6 3.6028(16) 5_656 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O7 T1 O1 111.03(6) . . ? 
O7 T1 O6 109.87(8) . . ? 
O1 T1 O6 110.32(5) . . ? 
O7 T1 O5 107.60(7) . . ? 
O1 T1 O5 111.93(5) . . ? 
O6 T1 O5 105.94(6) . . ? 
O7 T1 A2 52.4(5) . 7 ? 
O1 T1 A2 131.59(12) . 7 ? 
O6 T1 A2 118.09(12) . 7 ? 
O5 T1 A2 55.3(4) . 7 ? 
O7 T1 M3 78.80(6) . . ? 
O1 T1 M3 34.10(3) . . ? 
O6 T1 M3 134.64(4) . . ? 
O5 T1 M3 113.64(4) . . ? 
A2 T1 M3 102.6(3) 7 . ? 
O7 T1 M4 120.58(6) . 7_556 ? 
O1 T1 M4 128.36(4) . 7_556 ? 
O6 T1 M4 51.24(4) . 7_556 ? 
O5 T1 M4 54.73(4) . 7_556 ? 
A2 T1 M4 85.2(4) 7 7_556 ? 
M3 T1 M4 158.671(18) . 7_556 ? 
O7 T1 M1 110.22(5) . . ? 
O1 T1 M1 33.04(3) . . ? 
O6 T1 M1 80.53(4) . . ? 
O5 T1 M1 136.53(4) . . ? 
A2 T1 M1 156.9(4) 7 . ? 
M3 T1 M1 55.650(12) . . ? 
M4 T1 M1 117.942(15) 7_556 . ? 
O7 T1 O4 168.03(7) . 7_556 ? 
O1 T1 O4 63.64(4) . 7_556 ? 
O6 T1 O4 82.08(4) . 7_556 ? 
O5 T1 O4 67.03(4) . 7_556 ? 
A2 T1 O4 121.9(4) 7 7_556 ? 
M3 T1 O4 93.40(2) . 7_556 ? 
M4 T1 O4 65.96(2) 7_556 7_556 ? 
M1 T1 O4 71.609(19) . 7_556 ? 
O7 T1 A1 44.12(7) . 5_655 ? 
O1 T1 A1 122.63(11) . 5_655 ? 
O6 T1 A1 126.23(12) . 5_655 ? 
O5 T1 A1 63.81(6) . 5_655 ? 
A2 T1 A1 11.8(4) 7 5_655 ? 
M3 T1 A1 91.71(10) . 5_655 ? 
M4 T1 A1 97.00(8) 7_556 5_655 ? 
M1 T1 A1 145.06(8) . 5_655 ? 
O4 T1 A1 128.18(6) 7_556 5_655 ? 
O7 T1 A1 41.69(7) . . ? 
O1 T1 A1 133.89(11) . . ? 
O6 T1 A1 114.20(11) . . ? 
O5 T1 A1 66.57(6) . . ? 
A2 T1 A1 11.7(4) 7 . ? 
M3 T1 A1 101.53(9) . . ? 
M4 T1 A1 90.02(8) 7_556 . ? 
M1 T1 A1 150.45(6) . . ? 
O4 T1 A1 133.45(6) 7_556 . ? 
A1 T1 A1 12.2(2) 5_655 . ? 
O7 T1 A2 34.3(3) . 3_545 ? 
O1 T1 A2 124.59(16) . 3_545 ? 
O6 T1 A2 121.22(5) . 3_545 ? 
O5 T1 A2 73.4(3) . 3_545 ? 
A2 T1 A2 18.6(8) 7 3_545 ? 
M3 T1 A2 91.5(2) . 3_545 ? 
M4 T1 A2 100.5(3) 7_556 3_545 ? 
M1 T1 A2 140.3(3) . 3_545 ? 
O4 T1 A2 138.6(3) 7_556 3_545 ? 
A1 T1 A2 10.4(2) 5_655 3_545 ? 
A1 T1 A2 10.5(2) . 3_545 ? 
O4 T2 O2 116.78(5) . . ? 
O4 T2 O5 109.34(6) . 1_556 ? 
O2 T2 O5 109.42(5) . 1_556 ? 
O4 T2 O6 104.00(5) . . ? 
O2 T2 O6 108.39(5) . . ? 
O5 T2 O6 108.54(6) 1_556 . ? 
O4 T2 M4 48.50(4) . 7_556 ? 
O2 T2 M4 130.68(4) . 7_556 ? 
O5 T2 M4 119.87(4) 1_556 7_556 ? 
O6 T2 M4 55.54(4) . 7_556 ? 
O4 T2 M42 42.2(3) . 7_556 ? 
O2 T2 M42 128.92(11) . 7_556 ? 
O5 T2 M42 121.35(8) 1_556 7_556 ? 
O6 T2 M42 61.8(3) . 7_556 ? 
M4 T2 M42 6.6(3) 7_556 7_556 ? 
O4 T2 A2 116.7(3) . 7_556 ? 
O2 T2 A2 126.5(3) . 7_556 ? 
O5 T2 A2 52.22(8) 1_556 7_556 ? 
O6 T2 A2 56.42(10) . 7_556 ? 
M4 T2 A2 85.98(16) 7_556 7_556 ? 
M42 T2 A2 91.5(3) 7_556 7_556 ? 
O4 T2 O4 88.36(4) . 7_557 ? 
O2 T2 O4 63.30(4) . 7_557 ? 
O5 T2 O4 68.11(4) 1_556 7_557 ? 
O6 T2 O4 167.51(4) . 7_557 ? 
M4 T2 O4 136.86(3) 7_556 7_557 ? 
M42 T2 O4 130.5(3) 7_556 7_557 ? 
A2 T2 O4 119.68(3) 7_556 7_557 ? 
O4 T2 O4 71.25(5) . 7_556 ? 
O2 T2 O4 65.31(4) . 7_556 ? 
O5 T2 O4 173.52(4) 1_556 7_556 ? 
O6 T2 O4 77.26(5) . 7_556 ? 
M4 T2 O4 65.60(2) 7_556 7_556 ? 
M42 T2 O4 63.64(9) 7_556 7_556 ? 
A2 T2 O4 133.68(9) 7_556 7_556 ? 
O4 T2 O4 105.59(3) 7_557 7_556 ? 
O4 T2 M4 78.85(4) . . ? 
O2 T2 M4 38.69(4) . . ? 
O5 T2 M4 133.77(4) 1_556 . ? 
O6 T2 M4 113.34(4) . . ? 
M4 T2 M4 99.888(14) 7_556 . ? 
M42 T2 M4 95.7(2) 7_556 . ? 
A2 T2 M4 162.1(3) 7_556 . ? 
O4 T2 M4 66.74(2) 7_557 . ? 
O4 T2 M4 39.745(17) 7_556 . ? 
O4 T2 O4 49.99(5) . 2_657 ? 
O2 T2 O4 150.88(4) . 2_657 ? 
O5 T2 O4 63.34(4) 1_556 2_657 ? 
O6 T2 O4 100.47(4) . 2_657 ? 
M4 T2 O4 64.45(2) 7_556 2_657 ? 
M42 T2 O4 62.69(8) 7_556 2_657 ? 
A2 T2 O4 73.4(3) 7_556 2_657 ? 
O4 T2 O4 88.82(3) 7_557 2_657 ? 
O4 T2 O4 119.16(2) 7_556 2_657 ? 
M4 T2 O4 124.37(2) . 2_657 ? 
O4 T2 O7 139.04(5) . 1_556 ? 
O2 T2 O7 96.20(4) . 1_556 ? 
O5 T2 O7 32.09(4) 1_556 1_556 ? 
O6 T2 O7 86.27(5) . 1_556 ? 
M4 T2 O7 124.72(3) 7_556 1_556 ? 
M42 T2 O7 129.8(3) 7_556 1_556 ? 
A2 T2 O7 38.90(14) 7_556 1_556 ? 
O4 T2 O7 85.49(3) 7_557 1_556 ? 
O4 T2 O7 148.98(3) 7_556 1_556 ? 
M4 T2 O7 133.66(3) . 1_556 ? 
O4 T2 O7 89.37(3) 2_657 1_556 ? 
O3 M1 O3 85.05(7) 5_556 . ? 
O3 M1 O1 84.90(5) 5_556 . ? 
O3 M1 O1 100.26(5) . . ? 
O3 M1 O1 100.26(5) 5_556 2_556 ? 
O3 M1 O1 84.90(5) . 2_556 ? 
O1 M1 O1 173.07(6) . 2_556 ? 
O3 M1 O2 177.71(5) 5_556 . ? 
O3 M1 O2 96.36(4) . . ? 
O1 M1 O2 93.06(4) . . ? 
O1 M1 O2 81.69(4) 2_556 . ? 
O3 M1 O2 96.36(4) 5_556 2_556 ? 
O3 M1 O2 177.71(5) . 2_556 ? 
O1 M1 O2 81.69(4) . 2_556 ? 
O1 M1 O2 93.06(4) 2_556 2_556 ? 
O2 M1 O2 82.29(5) . 2_556 ? 
O3 M1 M11 42.53(4) 5_556 5_556 ? 
O3 M1 M11 42.53(4) . 5_556 ? 
O1 M1 M11 93.47(3) . 5_556 ? 
O1 M1 M11 93.47(3) 2_556 5_556 ? 
O2 M1 M11 138.85(3) . 5_556 ? 
O2 M1 M11 138.85(3) 2_556 5_556 ? 
O3 M1 M1 42.53(4) 5_556 5_556 ? 
O3 M1 M1 42.53(4) . 5_556 ? 
O1 M1 M1 93.47(3) . 5_556 ? 
O1 M1 M1 93.47(3) 2_556 5_556 ? 
O2 M1 M1 138.85(3) . 5_556 ? 
O2 M1 M1 138.85(3) 2_556 5_556 ? 
M11 M1 M1 0.0 5_556 5_556 ? 
O3 M1 M3 41.93(4) 5_556 . ? 
O3 M1 M3 92.43(4) . . ? 
O1 M1 M3 42.99(3) . . ? 
O1 M1 M3 142.10(3) 2_556 . ? 
O2 M1 M3 136.05(2) . . ? 
O2 M1 M3 89.82(3) 2_556 . ? 
M11 M1 M3 61.579(9) 5_556 . ? 
M1 M1 M3 61.579(9) 5_556 . ? 
O3 M1 M33 92.43(4) 5_556 1_556 ? 
O3 M1 M33 41.93(4) . 1_556 ? 
O1 M1 M33 142.10(3) . 1_556 ? 
O1 M1 M33 42.99(3) 2_556 1_556 ? 
O2 M1 M33 89.82(3) . 1_556 ? 
O2 M1 M33 136.05(2) 2_556 1_556 ? 
M11 M1 M33 61.579(9) 5_556 1_556 ? 
M1 M1 M33 61.579(9) 5_556 1_556 ? 
M3 M1 M33 123.158(19) . 1_556 ? 
O3 M1 M3 92.43(4) 5_556 1_556 ? 
O3 M1 M3 41.93(4) . 1_556 ? 
O1 M1 M3 142.10(3) . 1_556 ? 
O1 M1 M3 42.99(3) 2_556 1_556 ? 
O2 M1 M3 89.82(3) . 1_556 ? 
O2 M1 M3 136.05(2) 2_556 1_556 ? 
M11 M1 M3 61.579(9) 5_556 1_556 ? 
M1 M1 M3 61.579(9) 5_556 1_556 ? 
M3 M1 M3 123.158(19) . 1_556 ? 
M33 M1 M3 0.0 1_556 1_556 ? 
O4 M2 O4 98.64(6) 7_556 8_454 ? 
O4 M2 O2 93.31(4) 7_556 2_556 ? 
O4 M2 O2 90.93(4) 8_454 2_556 ? 
O4 M2 O2 90.93(4) 7_556 1_554 ? 
O4 M2 O2 93.31(4) 8_454 1_554 ? 
O2 M2 O2 173.49(6) 2_556 1_554 ? 
O4 M2 O1 168.03(4) 7_556 2 ? 
O4 M2 O1 91.51(4) 8_454 2 ? 
O2 M2 O1 92.84(4) 2_556 2 ? 
O2 M2 O1 82.12(4) 1_554 2 ? 
O4 M2 O1 91.51(4) 7_556 . ? 
O4 M2 O1 168.03(4) 8_454 . ? 
O2 M2 O1 82.12(4) 2_556 . ? 
O2 M2 O1 92.84(4) 1_554 . ? 
O1 M2 O1 79.18(6) 2 . ? 
O4 M2 M42 49.17(18) 7_556 . ? 
O4 M2 M42 91.7(3) 8_454 . ? 
O2 M2 M42 44.6(2) 2_556 . ? 
O2 M2 M42 140.07(19) 1_554 . ? 
O1 M2 M42 137.3(2) 2 . ? 
O1 M2 M42 90.2(3) . . ? 
O4 M2 M42 91.7(3) 7_556 1_554 ? 
O4 M2 M42 49.17(18) 8_454 1_554 ? 
O2 M2 M42 140.07(19) 2_556 1_554 ? 
O2 M2 M42 44.6(2) 1_554 1_554 ? 
O1 M2 M42 90.2(3) 2 1_554 ? 
O1 M2 M42 137.3(2) . 1_554 ? 
M42 M2 M42 122.8(7) . 1_554 ? 
O4 M2 M11 133.19(3) 7_556 1_554 ? 
O4 M2 M11 92.03(3) 8_454 1_554 ? 
O2 M2 M11 132.15(3) 2_556 1_554 ? 
O2 M2 M11 42.79(3) 1_554 1_554 ? 
O1 M2 M11 39.35(2) 2 1_554 ? 
O1 M2 M11 85.54(3) . 1_554 ? 
M42 M2 M11 175.1(3) . 1_554 ? 
M42 M2 M11 62.1(3) 1_554 1_554 ? 
O4 M2 M1 133.19(3) 7_556 1_554 ? 
O4 M2 M1 92.03(3) 8_454 1_554 ? 
O2 M2 M1 132.15(3) 2_556 1_554 ? 
O2 M2 M1 42.79(3) 1_554 1_554 ? 
O1 M2 M1 39.35(2) 2 1_554 ? 
O1 M2 M1 85.54(3) . 1_554 ? 
M42 M2 M1 175.1(3) . 1_554 ? 
M42 M2 M1 62.1(3) 1_554 1_554 ? 
M11 M2 M1 0.000(12) 1_554 1_554 ? 
O4 M2 M1 92.03(3) 7_556 . ? 
O4 M2 M1 133.19(3) 8_454 . ? 
O2 M2 M1 42.79(3) 2_556 . ? 
O2 M2 M1 132.15(3) 1_554 . ? 
O1 M2 M1 85.54(3) 2 . ? 
O1 M2 M1 39.35(2) . . ? 
M42 M2 M1 62.1(3) . . ? 
M42 M2 M1 175.1(3) 1_554 . ? 
M11 M2 M1 112.97(2) 1_554 . ? 
M1 M2 M1 112.97(2) 1_554 . ? 
O3 M3 O3 180.00(6) 5_556 1_554 ? 
O3 M3 O1 97.75(4) 5_556 5 ? 
O3 M3 O1 82.25(4) 1_554 5 ? 
O3 M3 O1 82.25(4) 5_556 . ? 
O3 M3 O1 97.75(4) 1_554 . ? 
O1 M3 O1 180.00(6) 5 . ? 
O3 M3 O1 82.25(4) 5_556 6 ? 
O3 M3 O1 97.75(4) 1_554 6 ? 
O1 M3 O1 81.79(6) 5 6 ? 
O1 M3 O1 98.21(6) . 6 ? 
O3 M3 O1 97.75(4) 5_556 2 ? 
O3 M3 O1 82.25(4) 1_554 2 ? 
O1 M3 O1 98.21(6) 5 2 ? 
O1 M3 O1 81.79(6) . 2 ? 
O1 M3 O1 180.00(6) 6 2 ? 
O3 M3 M11 140.29(3) 5_556 5 ? 
O3 M3 M11 39.71(3) 1_554 5 ? 
O1 M3 M11 42.55(2) 5 5 ? 
O1 M3 M11 137.45(2) . 5 ? 
O1 M3 M11 90.98(3) 6 5 ? 
O1 M3 M11 89.02(3) 2 5 ? 
O3 M3 M1 140.29(3) 5_556 5 ? 
O3 M3 M1 39.71(3) 1_554 5 ? 
O1 M3 M1 42.55(2) 5 5 ? 
O1 M3 M1 137.45(2) . 5 ? 
O1 M3 M1 90.98(3) 6 5 ? 
O1 M3 M1 89.02(3) 2 5 ? 
M11 M3 M1 0.000(14) 5 5 ? 
O3 M3 M1 39.71(3) 5_556 . ? 
O3 M3 M1 140.29(3) 1_554 . ? 
O1 M3 M1 137.45(2) 5 . ? 
O1 M3 M1 42.55(2) . . ? 
O1 M3 M1 89.02(3) 6 . ? 
O1 M3 M1 90.98(3) 2 . ? 
M11 M3 M1 180.000(14) 5 . ? 
M1 M3 M1 180.000(14) 5 . ? 
O3 M3 M11 39.71(3) 5_556 5_556 ? 
O3 M3 M11 140.29(3) 1_554 5_556 ? 
O1 M3 M11 90.98(3) 5 5_556 ? 
O1 M3 M11 89.02(3) . 5_556 ? 
O1 M3 M11 42.55(2) 6 5_556 ? 
O1 M3 M11 137.45(2) 2 5_556 ? 
M11 M3 M11 123.158(19) 5 5_556 ? 
M1 M3 M11 123.158(19) 5 5_556 ? 
M1 M3 M11 56.842(19) . 5_556 ? 
O3 M3 M1 39.71(3) 5_556 5_556 ? 
O3 M3 M1 140.29(3) 1_554 5_556 ? 
O1 M3 M1 90.98(3) 5 5_556 ? 
O1 M3 M1 89.02(3) . 5_556 ? 
O1 M3 M1 42.55(2) 6 5_556 ? 
O1 M3 M1 137.45(2) 2 5_556 ? 
M11 M3 M1 123.158(19) 5 5_556 ? 
M1 M3 M1 123.158(19) 5 5_556 ? 
M1 M3 M1 56.842(19) . 5_556 ? 
M11 M3 M1 0.000(14) 5_556 5_556 ? 
O4 M4 O4 153.20(7) 7_556 8_455 ? 
O4 M4 O2 76.67(4) 7_556 2_556 ? 
O4 M4 O2 81.77(4) 8_455 2_556 ? 
O4 M4 O2 81.77(4) 7_556 . ? 
O4 M4 O2 76.67(4) 8_455 . ? 
O2 M4 O2 72.59(6) 2_556 . ? 
O4 M4 O6 63.50(3) 7_556 7_556 ? 
O4 M4 O6 141.77(5) 8_455 7_556 ? 
O2 M4 O6 135.25(3) 2_556 7_556 ? 
O2 M4 O6 118.01(3) . 7_556 ? 
O4 M4 O6 141.77(5) 7_556 8_455 ? 
O4 M4 O6 63.50(3) 8_455 8_455 ? 
O2 M4 O6 118.01(3) 2_556 8_455 ? 
O2 M4 O6 135.25(3) . 8_455 ? 
O6 M4 O6 85.91(5) 7_556 8_455 ? 
O4 M4 O5 110.45(4) 7_556 7_556 ? 
O4 M4 O5 84.70(4) 8_455 7_556 ? 
O2 M4 O5 158.37(4) 2_556 7_556 ? 
O2 M4 O5 87.94(3) . 7_556 ? 
O6 M4 O5 62.37(4) 7_556 7_556 ? 
O6 M4 O5 69.66(4) 8_455 7_556 ? 
O4 M4 O5 84.70(4) 7_556 8_455 ? 
O4 M4 O5 110.45(4) 8_455 8_455 ? 
O2 M4 O5 87.94(3) 2_556 8_455 ? 
O2 M4 O5 158.37(4) . 8_455 ? 
O6 M4 O5 69.66(4) 7_556 8_455 ? 
O6 M4 O5 62.37(4) 8_455 8_455 ? 
O5 M4 O5 112.67(6) 7_556 8_455 ? 
O4 M4 T2 30.95(2) 7_556 7_556 ? 
O4 M4 T2 171.86(3) 8_455 7_556 ? 
O2 M4 T2 105.29(3) 2_556 7_556 ? 
O2 M4 T2 101.33(2) . 7_556 ? 
O6 M4 T2 32.57(2) 7_556 7_556 ? 
O6 M4 T2 115.14(4) 8_455 7_556 ? 
O5 M4 T2 87.36(3) 7_556 7_556 ? 
O5 M4 T2 74.31(3) 8_455 7_556 ? 
O4 M4 T2 171.86(3) 7_556 8_455 ? 
O4 M4 T2 30.95(2) 8_455 8_455 ? 
O2 M4 T2 101.33(2) 2_556 8_455 ? 
O2 M4 T2 105.29(3) . 8_455 ? 
O6 M4 T2 115.14(4) 7_556 8_455 ? 
O6 M4 T2 32.57(2) 8_455 8_455 ? 
O5 M4 T2 74.31(3) 7_556 8_455 ? 
O5 M4 T2 87.36(3) 8_455 8_455 ? 
T2 M4 T2 146.82(4) 7_556 8_455 ? 
O4 M4 M2 37.54(3) 7_556 . ? 
O4 M4 M2 121.98(4) 8_455 . ? 
O2 M4 M2 40.34(2) 2_556 . ? 
O2 M4 M2 81.17(4) . . ? 
O6 M4 M2 95.87(2) 7_556 . ? 
O6 M4 M2 136.82(3) 8_455 . ? 
O5 M4 M2 147.21(2) 7_556 . ? 
O5 M4 M2 77.82(3) 8_455 . ? 
T2 M4 M2 64.947(13) 7_556 . ? 
T2 M4 M2 138.401(17) 8_455 . ? 
O2 M42 O2 84.9(7) 2_556 . ? 
O2 M42 O4 90.0(4) 2_556 8_455 ? 
O2 M42 O4 84.1(4) . 8_455 ? 
O2 M42 O4 84.1(4) 2_556 7_556 ? 
O2 M42 O4 90.0(4) . 7_556 ? 
O4 M42 O4 172.0(10) 8_455 7_556 ? 
O2 M42 M2 43.65(18) 2_556 . ? 
O2 M42 M2 90.9(6) . . ? 
O4 M42 M2 133.6(6) 8_455 . ? 
O4 M42 M2 40.81(16) 7_556 . ? 
O2 M42 M22 90.9(6) 2_556 1_556 ? 
O2 M42 M22 43.65(18) . 1_556 ? 
O4 M42 M22 40.81(16) 8_455 1_556 ? 
O4 M42 M22 133.6(6) 7_556 1_556 ? 
M2 M42 M22 122.8(7) . 1_556 ? 
O2 M42 M2 90.9(6) 2_556 1_556 ? 
O2 M42 M2 43.65(18) . 1_556 ? 
O4 M42 M2 40.81(16) 8_455 1_556 ? 
O4 M42 M2 133.6(6) 7_556 1_556 ? 
M2 M42 M2 122.8(7) . 1_556 ? 
M22 M42 M2 0.000(15) 1_556 1_556 ? 
O2 M42 M1 42.4(4) 2_556 . ? 
O2 M42 M1 42.4(4) . . ? 
O4 M42 M1 86.0(5) 8_455 . ? 
O4 M42 M1 86.0(5) 7_556 . ? 
M2 M42 M1 61.4(3) . . ? 
M22 M42 M1 61.4(3) 1_556 . ? 
M2 M42 M1 61.4(3) 1_556 . ? 
O2 M42 T2 109.09(15) 2_556 7_556 ? 
O2 M42 T2 104.69(13) . 7_556 ? 
O4 M42 T2 159.4(8) 8_455 7_556 ? 
O4 M42 T2 28.22(17) 7_556 7_556 ? 
M2 M42 T2 65.746(14) . 7_556 ? 
M22 M42 T2 141.96(9) 1_556 7_556 ? 
M2 M42 T2 141.96(9) 1_556 7_556 ? 
M1 M42 T2 113.2(3) . 7_556 ? 
O2 M42 T2 104.69(13) 2_556 8_455 ? 
O2 M42 T2 109.09(15) . 8_455 ? 
O4 M42 T2 28.22(17) 8_455 8_455 ? 
O4 M42 T2 159.4(8) 7_556 8_455 ? 
M2 M42 T2 141.96(9) . 8_455 ? 
M22 M42 T2 65.746(15) 1_556 8_455 ? 
M2 M42 T2 65.746(15) 1_556 8_455 ? 
M1 M42 T2 113.2(3) . 8_455 ? 
T2 M42 T2 133.7(7) 7_556 8_455 ? 
A2 A1 A2 120(3) 3_545 7 ? 
A2 A1 A1 59.8(13) 3_545 5_655 ? 
A2 A1 A1 59.8(13) 7 5_655 ? 
A2 A1 O7 87.8(5) 3_545 . ? 
A2 A1 O7 87.8(5) 7 . ? 
A1 A1 O7 85.7(10) 5_655 . ? 
A2 A1 O7 83.7(5) 3_545 5_655 ? 
A2 A1 O7 83.7(5) 7 5_655 ? 
A1 A1 O7 77.5(9) 5_655 5_655 ? 
O7 A1 O7 163.1(3) . 5_655 ? 
A2 A1 O6 167.8(12) 3_545 2_656 ? 
A2 A1 O6 71.0(13) 7 2_656 ? 
A1 A1 O6 130.40(19) 5_655 2_656 ? 
O7 A1 O6 86.63(14) . 2_656 ? 
O7 A1 O6 104.24(18) 5_655 2_656 ? 
A2 A1 O6 71.0(13) 3_545 5_656 ? 
A2 A1 O6 167.8(12) 7 5_656 ? 
A1 A1 O6 130.40(19) 5_655 5_656 ? 
O7 A1 O6 86.63(14) . 5_656 ? 
O7 A1 O6 104.24(18) 5_655 5_656 ? 
O6 A1 O6 97.84(19) 2_656 5_656 ? 
A2 A1 T1 64.1(5) 3_545 5_655 ? 
A2 A1 T1 110.7(6) 7 5_655 ? 
A1 A1 T1 85.3(8) 5_655 5_655 ? 
O7 A1 T1 151.24(10) . 5_655 ? 
O7 A1 T1 28.08(5) 5_655 5_655 ? 
O6 A1 T1 119.6(2) 2_656 5_655 ? 
O6 A1 T1 78.72(10) 5_656 5_655 ? 
A2 A1 T1 110.7(6) 3_545 2_655 ? 
A2 A1 T1 64.1(5) 7 2_655 ? 
A1 A1 T1 85.3(8) 5_655 2_655 ? 
O7 A1 T1 151.24(10) . 2_655 ? 
O7 A1 T1 28.08(5) 5_655 2_655 ? 
O6 A1 T1 78.72(10) 2_656 2_655 ? 
O6 A1 T1 119.6(2) 5_656 2_655 ? 
T1 A1 T1 54.43(9) 5_655 2_655 ? 
A2 A1 O7 116.5(11) 3_545 5_656 ? 
A2 A1 O7 116.5(11) 7 5_656 ? 
A1 A1 O7 152.4(10) 5_655 5_656 ? 
O7 A1 O7 66.75(14) . 5_656 ? 
O7 A1 O7 130.1(3) 5_655 5_656 ? 
O6 A1 O7 51.35(9) 2_656 5_656 ? 
O6 A1 O7 51.35(9) 5_656 5_656 ? 
T1 A1 O7 118.90(18) 5_655 5_656 ? 
T1 A1 O7 118.90(18) 2_655 5_656 ? 
A2 A1 T1 62.7(4) 3_545 6 ? 
A2 A1 T1 109.2(8) 7 6 ? 
A1 A1 T1 82.6(8) 5_655 6 ? 
O7 A1 T1 27.34(5) . 6 ? 
O7 A1 T1 146.30(14) 5_655 6 ? 
O6 A1 T1 109.37(16) 2_656 6 ? 
O6 A1 T1 69.25(9) 5_656 6 ? 
T1 A1 T1 124.15(4) 5_655 6 ? 
T1 A1 T1 167.8(2) 2_655 6 ? 
O7 A1 T1 72.94(11) 5_656 6 ? 
A2 A1 T1 109.2(8) 3_545 . ? 
A2 A1 T1 62.7(4) 7 . ? 
A1 A1 T1 82.6(8) 5_655 . ? 
O7 A1 T1 27.34(5) . . ? 
O7 A1 T1 146.30(14) 5_655 . ? 
O6 A1 T1 69.25(9) 2_656 . ? 
O6 A1 T1 109.37(16) 5_656 . ? 
T1 A1 T1 167.8(2) 5_655 . ? 
T1 A1 T1 124.15(4) 2_655 . ? 
O7 A1 T1 72.94(11) 5_656 . ? 
T1 A1 T1 54.14(9) 6 . ? 
A1 A2 A1 60(3) 3_455 7 ? 
A1 A2 A2 30.2(13) 3_455 5_565 ? 
A1 A2 A2 30.2(13) 7 5_565 ? 
A1 A2 O7 75.6(8) 3_455 3_455 ? 
A1 A2 O7 79.7(8) 7 3_455 ? 
A2 A2 O7 75.7(6) 5_565 3_455 ? 
A1 A2 O7 79.7(8) 3_455 7 ? 
A1 A2 O7 75.6(8) 7 7 ? 
A2 A2 O7 75.7(6) 5_565 7 ? 
O7 A2 O7 151.4(12) 3_455 7 ? 
A1 A2 O5 136.5(5) 3_455 8_455 ? 
A1 A2 O5 124.4(7) 7 8_455 ? 
A2 A2 O5 138.3(4) 5_565 8_455 ? 
O7 A2 O5 64.6(2) 3_455 8_455 ? 
O7 A2 O5 142.9(9) 7 8_455 ? 
A1 A2 O5 124.4(7) 3_455 7 ? 
A1 A2 O5 136.5(5) 7 7 ? 
A2 A2 O5 138.3(4) 5_565 7 ? 
O7 A2 O5 142.9(9) 3_455 7 ? 
O7 A2 O5 64.6(2) 7 7 ? 
O5 A2 O5 83.5(8) 8_455 7 ? 
A1 A2 O6 154.2(17) 3_455 8_454 ? 
A1 A2 O6 94.5(9) 7 8_454 ? 
A2 A2 O6 124.5(5) 5_565 8_454 ? 
O7 A2 O6 107.9(3) 3_455 8_454 ? 
O7 A2 O6 88.4(2) 7 8_454 ? 
O5 A2 O6 61.4(4) 8_455 8_454 ? 
O5 A2 O6 68.6(5) 7 8_454 ? 
A1 A2 O6 94.5(9) 3_455 7_556 ? 
A1 A2 O6 154.2(17) 7 7_556 ? 
A2 A2 O6 124.5(5) 5_565 7_556 ? 
O7 A2 O6 88.4(2) 3_455 7_556 ? 
O7 A2 O6 107.9(3) 7 7_556 ? 
O5 A2 O6 68.6(5) 8_455 7_556 ? 
O5 A2 O6 61.4(4) 7 7_556 ? 
O6 A2 O6 111.1(9) 8_454 7_556 ? 
A1 A2 T1 104.1(5) 3_455 7 ? 
A1 A2 T1 105.6(5) 7 7 ? 
A2 A2 T1 107.2(5) 5_565 7 ? 
O7 A2 T1 173.8(5) 3_455 7 ? 
O7 A2 T1 32.05(13) 7 7 ? 
O5 A2 T1 113.6(8) 8_455 7 ? 
O5 A2 T1 32.64(9) 7 7 ? 
O6 A2 T1 75.2(3) 8_454 7 ? 
O6 A2 T1 85.4(4) 7_556 7 ? 
A1 A2 T1 105.6(5) 3_455 8_455 ? 
A1 A2 T1 104.1(5) 7 8_455 ? 
A2 A2 T1 107.2(5) 5_565 8_455 ? 
O7 A2 T1 32.05(13) 3_455 8_455 ? 
O7 A2 T1 173.8(5) 7 8_455 ? 
O5 A2 T1 32.64(9) 8_455 8_455 ? 
O5 A2 T1 113.6(8) 7 8_455 ? 
O6 A2 T1 85.4(4) 8_454 8_455 ? 
O6 A2 T1 75.2(3) 7_556 8_455 ? 
T1 A2 T1 145.5(9) 7 8_455 ? 
A1 A2 T2 161.7(8) 3_455 8_454 ? 
A1 A2 T2 113.1(10) 7 8_454 ? 
A2 A2 T2 140.9(3) 5_565 8_454 ? 
O7 A2 T2 86.6(3) 3_455 8_454 ? 
O7 A2 T2 116.3(5) 7 8_454 ? 
O5 A2 T2 30.4(2) 8_455 8_454 ? 
O5 A2 T2 72.8(6) 7 8_454 ? 
O6 A2 T2 31.0(2) 8_454 8_454 ? 
O6 A2 T2 88.8(7) 7_556 8_454 ? 
T1 A2 T2 94.1(6) 7 8_454 ? 
T1 A2 T2 57.9(3) 8_455 8_454 ? 
T1 O1 M1 120.41(6) . . ? 
T1 O1 M3 118.77(5) . . ? 
M1 O1 M3 94.46(4) . . ? 
T1 O1 M2 119.19(5) . . ? 
M1 O1 M2 99.60(4) . . ? 
M3 O1 M2 99.52(5) . . ? 
T1 O1 O7 34.30(3) . . ? 
M1 O1 O7 117.45(5) . . ? 
M3 O1 O7 86.20(4) . . ? 
M2 O1 O7 142.05(5) . . ? 
T1 O1 O4 85.54(4) . 7_556 ? 
M1 O1 O4 98.00(4) . 7_556 ? 
M3 O1 O4 141.26(5) . 7_556 ? 
M2 O1 O4 42.28(3) . 7_556 ? 
O7 O1 O4 119.07(4) . 7_556 ? 
T1 O1 O4 124.88(4) . 8_454 ? 
M1 O1 O4 96.40(4) . 8_454 ? 
M3 O1 O4 95.04(4) . 8_454 ? 
M2 O1 O4 5.77(2) . 8_454 ? 
O7 O1 O4 145.97(5) . 8_454 ? 
O4 O1 O4 47.26(4) 7_556 8_454 ? 
T1 O1 O4 58.24(3) . . ? 
M1 O1 O4 81.85(3) . . ? 
M3 O1 O4 171.94(4) . . ? 
M2 O1 O4 88.19(3) . . ? 
O7 O1 O4 89.16(4) . . ? 
O4 O1 O4 46.71(4) 7_556 . ? 
O4 O1 O4 92.49(2) 8_454 . ? 
T1 O1 O7 152.43(5) . 5 ? 
M1 O1 O7 78.62(4) . 5 ? 
M3 O1 O7 34.87(2) . 5 ? 
M2 O1 O7 71.95(3) . 5 ? 
O7 O1 O7 121.06(4) . 5 ? 
O4 O1 O7 113.03(4) 7_556 5 ? 
O4 O1 O7 66.46(2) 8_454 5 ? 
O4 O1 O7 149.14(3) . 5 ? 
T2 O2 M22 122.54(6) . 1_556 ? 
T2 O2 M2 122.54(6) . 1_556 ? 
M22 O2 M2 0.0 1_556 1_556 ? 
T2 O2 M42 120.5(3) . . ? 
M22 O2 M42 91.78(6) 1_556 . ? 
M2 O2 M42 91.78(6) 1_556 . ? 
T2 O2 M1 121.99(5) . . ? 
M22 O2 M1 96.54(4) 1_556 . ? 
M2 O2 M1 96.54(4) 1_556 . ? 
M42 O2 M1 96.4(4) . . ? 
T2 O2 M4 116.17(5) . . ? 
M22 O2 M4 91.05(4) 1_556 . ? 
M2 O2 M4 91.05(4) 1_556 . ? 
M42 O2 M4 6.1(4) . . ? 
M1 O2 M4 102.56(4) . . ? 
T2 O2 O4 31.24(3) . . ? 
M22 O2 O4 121.09(5) 1_556 . ? 
M2 O2 O4 121.09(5) 1_556 . ? 
M42 O2 O4 90.4(3) . . ? 
M1 O2 O4 141.56(4) . . ? 
M4 O2 O4 85.54(4) . . ? 
T2 O2 O4 86.24(5) . 7_557 ? 
M22 O2 O4 42.98(3) 1_556 7_557 ? 
M2 O2 O4 42.98(3) 1_556 7_557 ? 
M42 O2 O4 92.3(3) . 7_557 ? 
M1 O2 O4 138.93(4) . 7_557 ? 
M4 O2 O4 87.60(4) . 7_557 ? 
O4 O2 O4 78.10(4) . 7_557 ? 
T2 O2 O4 143.43(6) . 8_455 ? 
M22 O2 O4 41.85(3) 1_556 8_455 ? 
M2 O2 O4 41.85(3) 1_556 8_455 ? 
M42 O2 O4 50.33(3) . 8_455 ? 
M1 O2 O4 94.48(4) . 8_455 ? 
M4 O2 O4 50.54(3) . 8_455 ? 
O4 O2 O4 118.15(3) . 8_455 ? 
O4 O2 O4 61.58(4) 7_557 8_455 ? 
T2 O2 O4 86.07(4) . 7_556 ? 
M22 O2 O4 138.93(5) 1_556 7_556 ? 
M2 O2 O4 138.93(5) 1_556 7_556 ? 
M42 O2 O4 47.16(5) . 7_556 ? 
M1 O2 O4 90.05(4) . 7_556 ? 
M4 O2 O4 48.09(3) . 7_556 ? 
O4 O2 O4 67.43(4) . 7_556 ? 
O4 O2 O4 123.74(5) 7_557 7_556 ? 
O4 O2 O4 97.34(4) 8_455 7_556 ? 
T2 O2 O7 62.19(4) . 1_556 ? 
M22 O2 O7 81.39(4) 1_556 1_556 ? 
M2 O2 O7 81.39(4) 1_556 1_556 ? 
M42 O2 O7 172.71(18) . 1_556 ? 
M1 O2 O7 86.96(3) . 1_556 ? 
M4 O2 O7 168.52(4) . 1_556 ? 
O4 O2 O7 90.95(4) . 1_556 ? 
O4 O2 O7 80.97(4) 7_557 1_556 ? 
O4 O2 O7 123.10(4) 8_455 1_556 ? 
O4 O2 O7 139.56(4) 7_556 1_556 ? 
M11 O3 M1 0.000(16) 5_556 5_556 ? 
M11 O3 M1 94.95(7) 5_556 . ? 
M1 O3 M1 94.95(7) 5_556 . ? 
M11 O3 M33 98.35(5) 5_556 1_556 ? 
M1 O3 M33 98.35(5) 5_556 1_556 ? 
M1 O3 M33 98.35(5) . 1_556 ? 
M11 O3 M3 98.35(5) 5_556 1_556 ? 
M1 O3 M3 98.35(5) 5_556 1_556 ? 
M1 O3 M3 98.35(5) . 1_556 ? 
M33 O3 M3 0.0 1_556 1_556 ? 
M11 O3 O7 132.34(4) 5_556 1_556 ? 
M1 O3 O7 132.34(4) 5_556 1_556 ? 
M1 O3 O7 132.34(4) . 1_556 ? 
M33 O3 O7 72.73(5) 1_556 1_556 ? 
M3 O3 O7 72.73(5) 1_556 1_556 ? 
M11 O3 O7 87.75(5) 5_556 . ? 
M1 O3 O7 87.75(5) 5_556 . ? 
M1 O3 O7 87.75(5) . . ? 
M33 O3 O7 170.91(7) 1_556 . ? 
M3 O3 O7 170.91(7) 1_556 . ? 
O7 O3 O7 98.18(5) 1_556 . ? 
M11 O3 O7 68.29(4) 5_556 5_556 ? 
M1 O3 O7 68.29(4) 5_556 5_556 ? 
M1 O3 O7 68.29(4) . 5_556 ? 
M33 O3 O7 45.59(4) 1_556 5_556 ? 
M3 O3 O7 45.59(4) 1_556 5_556 ? 
O7 O3 O7 118.32(5) 1_556 5_556 ? 
O7 O3 O7 143.50(5) . 5_556 ? 
M11 O3 O4 38.68(3) 5_556 3_445 ? 
M1 O3 O4 38.68(3) 5_556 3_445 ? 
M1 O3 O4 120.51(5) . 3_445 ? 
M33 O3 O4 67.17(2) 1_556 3_445 ? 
M3 O3 O4 67.17(2) 1_556 3_445 ? 
O7 O3 O4 99.43(3) 1_556 3_445 ? 
O7 O3 O4 115.42(2) . 3_445 ? 
O7 O3 O4 61.304(18) 5_556 3_445 ? 
M11 O3 O4 120.51(5) 5_556 8_455 ? 
M1 O3 O4 120.51(5) 5_556 8_455 ? 
M1 O3 O4 38.68(3) . 8_455 ? 
M33 O3 O4 67.17(2) 1_556 8_455 ? 
M3 O3 O4 67.17(2) 1_556 8_455 ? 
O7 O3 O4 99.43(3) 1_556 8_455 ? 
O7 O3 O4 115.42(2) . 8_455 ? 
O7 O3 O4 61.304(18) 5_556 8_455 ? 
O4 O3 O4 121.89(3) 3_445 8_455 ? 
M11 O3 O4 152.81(5) 5_556 7_557 ? 
M1 O3 O4 152.81(5) 5_556 7_557 ? 
M1 O3 O4 67.09(3) . 7_557 ? 
M33 O3 O4 66.17(2) 1_556 7_557 ? 
M3 O3 O4 66.17(2) 1_556 7_557 ? 
O7 O3 O4 66.62(2) 1_556 7_557 ? 
O7 O3 O4 110.68(2) . 7_557 ? 
O7 O3 O4 85.66(2) 5_556 7_557 ? 
O4 O3 O4 133.34(3) 3_445 7_557 ? 
O4 O3 O4 33.85(3) 8_455 7_557 ? 
T2 O4 M22 141.34(7) . 7_556 ? 
T2 O4 M2 141.34(7) . 7_556 ? 
M22 O4 M2 0.00(2) 7_556 7_556 ? 
T2 O4 M42 109.6(5) . 7_556 ? 
M22 O4 M42 90.0(3) 7_556 7_556 ? 
M2 O4 M42 90.0(3) 7_556 7_556 ? 
T2 O4 M4 100.54(5) . 7_556 ? 
M22 O4 M4 96.14(4) 7_556 7_556 ? 
M2 O4 M4 96.14(4) 7_556 7_556 ? 
M42 O4 M4 9.4(5) 7_556 7_556 ? 
T2 O4 O6 38.65(3) . . ? 
M22 O4 O6 141.65(6) 7_556 . ? 
M2 O4 O6 141.65(6) 7_556 . ? 
M42 O4 O6 71.0(5) 7_556 . ? 
M4 O4 O6 61.93(4) 7_556 . ? 
T2 O4 O5 35.76(4) . 1_556 ? 
M22 O4 O5 105.58(5) 7_556 1_556 ? 
M2 O4 O5 105.58(5) 7_556 1_556 ? 
M42 O4 O5 120.7(5) 7_556 1_556 ? 
M4 O4 O5 112.02(5) 7_556 1_556 ? 
O6 O4 O5 61.64(4) . 1_556 ? 
T2 O4 O2 31.97(3) . . ? 
M22 O4 O2 147.98(5) 7_556 . ? 
M2 O4 O2 147.98(5) 7_556 . ? 
M42 O4 O2 122.0(3) 7_556 . ? 
M4 O4 O2 115.49(5) 7_556 . ? 
O6 O4 O2 59.97(3) . . ? 
O5 O4 O2 59.24(4) 1_556 . ? 
T2 O4 O2 106.73(5) . 7_557 ? 
M22 O4 O2 46.09(3) 7_556 7_557 ? 
M2 O4 O2 46.09(3) 7_556 7_557 ? 
M42 O4 O2 136.1(3) 7_556 7_557 ? 
M4 O4 O2 141.42(5) 7_556 7_557 ? 
O6 O4 O2 140.05(5) . 7_557 ? 
O5 O4 O2 78.45(4) 1_556 7_557 ? 
O2 O4 O2 101.90(4) . 7_557 ? 
T2 O4 O1 157.68(6) . 7_556 ? 
M22 O4 O1 46.21(3) 7_556 7_556 ? 
M2 O4 O1 46.21(3) 7_556 7_556 ? 
M42 O4 O1 89.2(5) 7_556 7_556 ? 
M4 O4 O1 98.61(4) 7_556 7_556 ? 
O6 O4 O1 156.83(5) . 7_556 ? 
O5 O4 O1 141.44(5) 1_556 7_556 ? 
O2 O4 O1 127.24(5) . 7_556 ? 
O2 O4 O1 63.00(3) 7_557 7_556 ? 
T2 O4 O2 146.36(6) . 8 ? 
M22 O4 O2 44.83(3) 7_556 8 ? 
M2 O4 O2 44.83(3) 7_556 8 ? 
M42 O4 O2 45.6(4) 7_556 8 ? 
M4 O4 O2 52.79(3) 7_556 8 ? 
O6 O4 O2 111.81(4) . 8 ? 
O5 O4 O2 128.02(5) 1_556 8 ? 
O2 O4 O2 166.81(6) . 8 ? 
O2 O4 O2 90.81(4) 7_557 8 ? 
O1 O4 O2 55.95(3) 7_556 8 ? 
T2 O4 O4 105.69(5) . 2_657 ? 
M22 O4 O4 40.68(3) 7_556 2_657 ? 
M2 O4 O4 40.68(3) 7_556 2_657 ? 
M42 O4 O4 86.58(5) 7_556 2_657 ? 
M4 O4 O4 86.66(5) 7_556 2_657 ? 
O6 O4 O4 103.44(4) . 2_657 ? 
O5 O4 O4 72.81(4) 1_556 2_657 ? 
O2 O4 O4 131.66(5) . 2_657 ? 
O2 O4 O4 60.17(4) 7_557 2_657 ? 
O1 O4 O4 86.72(3) 7_556 2_657 ? 
O2 O4 O4 58.25(4) 8 2_657 ? 
T2 O4 O5 102.13(5) . 7_556 ? 
M22 O4 O5 82.95(4) 7_556 7_556 ? 
M2 O4 O5 82.95(4) 7_556 7_556 ? 
M42 O4 O5 136.4(4) 7_556 7_556 ? 
M4 O4 O5 144.21(5) 7_556 7_556 ? 
O6 O4 O5 133.68(5) . 7_556 ? 
O5 O4 O5 102.53(4) 1_556 7_556 ? 
O2 O4 O5 74.39(4) . 7_556 ? 
O2 O4 O5 53.76(3) 7_557 7_556 ? 
O1 O4 O5 55.60(3) 7_556 7_556 ? 
O2 O4 O5 111.34(4) 8 7_556 ? 
O4 O4 O5 113.01(4) 2_657 7_556 ? 
T2 O4 O2 126.19(6) . 7_556 ? 
M22 O4 O2 91.02(4) 7_556 7_556 ? 
M2 O4 O2 91.02(4) 7_556 7_556 ? 
M42 O4 O2 42.9(4) 7_556 7_556 ? 
M4 O4 O2 50.14(3) 7_556 7_556 ? 
O6 O4 O2 96.10(4) . 7_556 ? 
O5 O4 O2 157.69(5) 1_556 7_556 ? 
O2 O4 O2 112.57(4) . 7_556 ? 
O2 O4 O2 123.74(5) 7_557 7_556 ? 
O1 O4 O2 60.76(3) 7_556 7_556 ? 
O2 O4 O2 56.17(4) 8 7_556 ? 
O4 O4 O2 114.27(5) 2_657 7_556 ? 
O5 O4 O2 94.07(4) 7_556 7_556 ? 
T2 O4 T2 91.64(4) . 7_557 ? 
M22 O4 T2 73.55(3) 7_556 7_557 ? 
M2 O4 T2 73.55(3) 7_556 7_557 ? 
M42 O4 T2 158.7(5) 7_556 7_557 ? 
M4 O4 T2 167.79(5) 7_556 7_557 ? 
O6 O4 T2 130.27(4) . 7_557 ? 
O5 O4 T2 77.67(4) 1_556 7_557 ? 
O2 O4 T2 75.53(3) . 7_557 ? 
O2 O4 T2 30.47(2) 7_557 7_557 ? 
O1 O4 T2 69.61(3) 7_556 7_557 ? 
O2 O4 T2 115.62(4) 8 7_557 ? 
O4 O4 T2 89.40(4) 2_657 7_557 ? 
O5 O4 T2 30.20(2) 7_556 7_557 ? 
O2 O4 T2 122.15(4) 7_556 7_557 ? 
T2 O4 T1 128.03(5) . 7_556 ? 
M22 O4 T1 72.92(3) 7_556 7_556 ? 
M2 O4 T1 72.92(3) 7_556 7_556 ? 
M42 O4 T1 106.3(5) 7_556 7_556 ? 
M4 O4 T1 114.93(4) 7_556 7_556 ? 
O6 O4 T1 143.55(5) . 7_556 ? 
O5 O4 T1 132.92(4) 1_556 7_556 ? 
O2 O4 T1 96.56(4) . 7_556 ? 
O2 O4 T1 67.32(3) 7_557 7_556 ? 
O1 O4 T1 30.82(2) 7_556 7_556 ? 
O2 O4 T1 85.01(3) 8 7_556 ? 
O4 O4 T1 112.78(2) 2_657 7_556 ? 
O5 O4 T1 30.71(2) 7_556 7_556 ? 
O2 O4 T1 65.79(3) 7_556 7_556 ? 
T2 O4 T1 56.36(2) 7_557 7_556 ? 
T2 O4 O4 81.07(5) . 7_556 ? 
M22 O4 O4 137.13(6) 7_556 7_556 ? 
M2 O4 O4 137.13(6) 7_556 7_556 ? 
M42 O4 O4 75.58(4) 7_556 7_556 ? 
M4 O4 O4 75.78(4) 7_556 7_556 ? 
O6 O4 O4 71.24(4) . 7_556 ? 
O5 O4 O4 116.57(5) 1_556 7_556 ? 
O2 O4 O4 61.33(4) . 7_556 ? 
O2 O4 O4 134.57(6) 7_557 7_556 ? 
O1 O4 O4 92.69(5) 7_556 7_556 ? 
O2 O4 O4 107.05(5) 8 7_556 ? 
O4 O4 O4 162.15(7) 2_657 7_556 ? 
O5 O4 O4 80.81(4) 7_556 7_556 ? 
O2 O4 O4 51.24(3) 7_556 7_556 ? 
T2 O4 O4 107.13(5) 7_557 7_556 ? 
T1 O4 O4 72.95(4) 7_556 7_556 ? 
T2 O4 O5 80.07(4) . 2_656 ? 
M22 O4 O5 83.71(4) 7_556 2_656 ? 
M2 O4 O5 83.71(4) 7_556 2_656 ? 
M42 O4 O5 57.3(3) 7_556 2_656 ? 
M4 O4 O5 51.37(3) 7_556 2_656 ? 
O6 O4 O5 57.94(3) . 2_656 ? 
O5 O4 O5 67.95(4) 1_556 2_656 ? 
O2 O4 O5 111.48(4) . 2_656 ? 
O2 O4 O5 107.11(4) 7_557 2_656 ? 
O1 O4 O5 121.27(4) 7_556 2_656 ? 
O2 O4 O5 67.23(3) 8 2_656 ? 
O4 O4 O5 48.93(3) 2_657 2_656 ? 
O5 O4 O5 160.74(5) 7_556 2_656 ? 
O2 O4 O5 100.00(4) 7_556 2_656 ? 
T2 O4 O5 131.52(4) 7_557 2_656 ? 
T1 O4 O5 151.89(4) 7_556 2_656 ? 
O4 O4 O5 118.31(5) 7_556 2_656 ? 
T2 O4 T2 108.75(5) . 7_556 ? 
M22 O4 T2 109.60(4) 7_556 7_556 ? 
M2 O4 T2 109.60(4) 7_556 7_556 ? 
M42 O4 T2 66.6(2) 7_556 7_556 ? 
M4 O4 T2 71.25(3) 7_556 7_556 ? 
O6 O4 T2 93.39(4) . 7_556 ? 
O5 O4 T2 144.12(5) 1_556 7_556 ? 
O2 O4 T2 86.50(4) . 7_556 ? 
O2 O4 T2 122.50(4) 7_557 7_556 ? 
O1 O4 T2 67.04(3) 7_556 7_556 ? 
O2 O4 T2 83.66(3) 8 7_556 ? 
O4 O4 T2 141.74(4) 2_657 7_556 ? 
O5 O4 T2 75.41(3) 7_556 7_556 ? 
O2 O4 T2 28.62(2) 7_556 7_556 ? 
T2 O4 T2 105.59(3) 7_557 7_556 ? 
T1 O4 T2 55.19(2) 7_556 7_556 ? 
O4 O4 T2 27.68(2) 7_556 7_556 ? 
O5 O4 T2 122.39(3) 2_656 7_556 ? 
T2 O4 O6 115.72(5) . 7_556 ? 
M22 O4 O6 96.41(4) 7_556 7_556 ? 
M2 O4 O6 96.41(4) 7_556 7_556 ? 
M42 O4 O6 90.4(3) 7_556 7_556 ? 
M4 O4 O6 96.73(4) 7_556 7_556 ? 
O6 O4 O6 116.06(4) . 7_556 ? 
O5 O4 O6 141.07(5) 1_556 7_556 ? 
O2 O4 O6 85.26(4) . 7_556 ? 
O2 O4 O6 95.45(4) 7_557 7_556 ? 
O1 O4 O6 50.22(3) 7_556 7_556 ? 
O2 O4 O6 90.09(3) 8 7_556 ? 
O4 O4 O6 136.89(2) 2_657 7_556 ? 
O5 O4 O6 48.27(3) 7_556 7_556 ? 
O2 O4 O6 47.69(3) 7_556 7_556 ? 
T2 O4 O6 78.36(3) 7_557 7_556 ? 
T1 O4 O6 28.72(2) 7_556 7_556 ? 
O4 O4 O6 44.82(3) 7_556 7_556 ? 
O5 O4 O6 147.66(4) 2_656 7_556 ? 
T2 O4 O6 27.863(19) 7_556 7_556 ? 
T2 O5 T1 134.62(7) 1_554 . ? 
T2 O5 A2 97.34(16) 1_554 7 ? 
T1 O5 A2 92.1(4) . 7 ? 
T2 O5 M4 122.81(6) 1_554 7_556 ? 
T1 O5 M4 93.91(5) . 7_556 ? 
A2 O5 M4 111.18(18) 7 7_556 ? 
T2 O5 O4 34.90(3) 1_554 1_554 ? 
T1 O5 O4 158.46(6) . 1_554 ? 
A2 O5 O4 107.0(3) 7 1_554 ? 
M4 O5 O4 88.49(4) 7_556 1_554 ? 
T2 O5 O7 129.03(7) 1_554 . ? 
T1 O5 O7 35.94(4) . . ? 
A2 O5 O7 56.2(4) 7 . ? 
M4 O5 O7 107.86(6) 7_556 . ? 
O4 O5 O7 159.60(6) 1_554 . ? 
T2 O5 O4 81.69(5) 1_554 7_556 ? 
T1 O5 O4 82.26(4) . 7_556 ? 
A2 O5 O4 170.7(3) 7 7_556 ? 
M4 O5 O4 76.69(4) 7_556 7_556 ? 
O4 O5 O4 77.47(4) 1_554 7_556 ? 
O7 O5 O4 117.45(5) . 7_556 ? 
T2 O5 O4 90.76(4) 1_554 2_656 ? 
T1 O5 O4 133.85(6) . 2_656 ? 
A2 O5 O4 89.1(4) 7 2_656 ? 
M4 O5 O4 43.93(3) 7_556 2_656 ? 
O4 O5 O4 58.26(4) 1_554 2_656 ? 
O7 O5 O4 126.55(5) . 2_656 ? 
O4 O5 O4 100.19(3) 7_556 2_656 ? 
T2 O5 O4 126.37(5) 1_554 . ? 
T1 O5 O4 71.05(4) . . ? 
A2 O5 O4 132.61(4) 7 . ? 
M4 O5 O4 32.417(19) 7_556 . ? 
O4 O5 O4 101.40(4) 1_554 . ? 
O7 O5 O4 98.89(5) . . ? 
O4 O5 O4 52.24(4) 7_556 . ? 
O4 O5 O4 74.63(3) 2_656 . ? 
T2 O5 O7 151.96(5) 1_554 5_656 ? 
T1 O5 O7 61.63(4) . 5_656 ? 
A2 O5 O7 55.78(10) 7 5_656 ? 
M4 O5 O7 68.21(3) 7_556 5_656 ? 
O4 O5 O7 137.93(4) 1_554 5_656 ? 
O7 O5 O7 45.82(5) . 5_656 ? 
O4 O5 O7 126.16(4) 7_556 5_656 ? 
O4 O5 O7 81.77(3) 2_656 5_656 ? 
O4 O5 O7 77.71(3) . 5_656 ? 
T2 O5 O7 82.71(4) 1_554 5_655 ? 
T1 O5 O7 110.13(4) . 5_655 ? 
A2 O5 O7 18.2(3) 7 5_655 ? 
M4 O5 O7 110.89(4) 7_556 5_655 ? 
O4 O5 O7 88.80(4) 1_554 5_655 ? 
O7 O5 O7 74.20(5) . 5_655 ? 
O4 O5 O7 164.32(4) 7_556 5_655 ? 
O4 O5 O7 78.43(3) 2_656 5_655 ? 
O4 O5 O7 139.83(4) . 5_655 ? 
O7 O5 O7 69.34(3) 5_656 5_655 ? 
T2 O5 O4 58.05(3) 1_554 8_454 ? 
T1 O5 O4 86.92(4) . 8_454 ? 
A2 O5 O4 139.56(17) 7 8_454 ? 
M4 O5 O4 109.22(3) 7_556 8_454 ? 
O4 O5 O4 72.13(3) 1_554 8_454 ? 
O7 O5 O4 112.00(4) . 8_454 ? 
O4 O5 O4 33.25(3) 7_556 8_454 ? 
O4 O5 O4 119.88(3) 2_656 8_454 ? 
O4 O5 O4 84.96(2) . 8_454 ? 
O7 O5 O4 147.56(3) 5_656 8_454 ? 
O7 O5 O4 134.75(4) 5_655 8_454 ? 
T2 O6 T1 136.79(7) . . ? 
T2 O6 M4 91.89(5) . 7_556 ? 
T1 O6 M4 97.72(5) . 7_556 ? 
T2 O6 O4 37.35(3) . . ? 
T1 O6 O4 131.24(6) . . ? 
M4 O6 O4 54.57(3) 7_556 . ? 
T2 O6 A2 92.6(3) . 7_556 ? 
T1 O6 A2 122.2(4) . 7_556 ? 
M4 O6 A2 110.6(3) 7_556 7_556 ? 
O4 O6 A2 105.9(5) . 7_556 ? 
T2 O6 O7 156.77(6) . . ? 
T1 O6 O7 34.87(4) . . ? 
M4 O6 O7 109.81(5) 7_556 . ? 
O4 O6 O7 162.00(6) . . ? 
A2 O6 O7 87.5(4) 7_556 . ? 
T2 O6 A1 101.70(11) . 5_656 ? 
T1 O6 A1 108.79(10) . 5_656 ? 
M4 O6 A1 120.89(13) 7_556 5_656 ? 
O4 O6 A1 119.80(10) . 5_656 ? 
A2 O6 A1 14.5(4) 7_556 5_656 ? 
O7 O6 A1 74.70(10) . 5_656 ? 
T2 O6 O4 74.87(4) . 7_556 ? 
T1 O6 O4 69.20(4) . 7_556 ? 
M4 O6 O4 70.28(3) 7_556 7_556 ? 
O4 O6 O4 63.94(4) . 7_556 ? 
A2 O6 O4 167.5(3) 7_556 7_556 ? 
O7 O6 O4 104.07(5) . 7_556 ? 
A1 O6 O4 168.68(13) 5_656 7_556 ? 
T2 O6 O7 131.14(6) . 5_656 ? 
T1 O6 O7 91.46(5) . 5_656 ? 
M4 O6 O7 87.43(3) 7_556 5_656 ? 
O4 O6 O7 121.83(5) . 5_656 ? 
A2 O6 O7 43.50(15) 7_556 5_656 ? 
O7 O6 O7 60.53(6) . 5_656 ? 
A1 O6 O7 41.78(12) 5_656 5_656 ? 
O4 O6 O7 147.35(4) 7_556 5_656 ? 
T2 O6 O7 70.42(4) . 1_556 ? 
T1 O6 O7 123.94(5) . 1_556 ? 
M4 O6 O7 134.83(4) 7_556 1_556 ? 
O4 O6 O7 99.80(4) . 1_556 ? 
A2 O6 O7 34.42(5) 7_556 1_556 ? 
O7 O6 O7 98.02(4) . 1_556 ? 
A1 O6 O7 34.75(12) 5_656 1_556 ? 
O4 O6 O7 136.62(4) 7_556 1_556 ? 
O7 O6 O7 75.95(4) 5_656 1_556 ? 
T2 O6 O4 57.69(4) . 2_657 ? 
T1 O6 O4 154.34(5) . 2_657 ? 
M4 O6 O4 57.40(3) 7_556 2_657 ? 
O4 O6 O4 41.69(4) . 2_657 ? 
A2 O6 O4 68.1(5) 7_556 2_657 ? 
O7 O6 O4 141.70(5) . 2_657 ? 
A1 O6 O4 82.56(10) 5_656 2_657 ? 
O4 O6 O4 103.94(3) 7_556 2_657 ? 
O7 O6 O4 81.96(3) 5_656 2_657 ? 
O7 O6 O4 78.60(3) 1_556 2_657 ? 
T2 O6 O4 109.92(5) . 2_656 ? 
T1 O6 O4 82.17(4) . 2_656 ? 
M4 O6 O4 18.33(2) 7_556 2_656 ? 
O4 O6 O4 72.57(4) . 2_656 ? 
A2 O6 O4 111.56(19) 7_556 2_656 ? 
O7 O6 O4 91.49(4) . 2_656 ? 
A1 O6 O4 117.72(13) 5_656 2_656 ? 
O4 O6 O4 73.39(2) 7_556 2_656 ? 
O7 O6 O4 78.21(3) 5_656 2_656 ? 
O7 O6 O4 143.23(4) 1_556 2_656 ? 
O4 O6 O4 72.23(3) 2_657 2_656 ? 
T1 O7 T1 135.36(10) 6 . ? 
T1 O7 A1 110.97(6) 6 . ? 
T1 O7 A1 110.97(6) . . ? 
T1 O7 A1 107.80(7) 6 5_655 ? 
T1 O7 A1 107.80(7) . 5_655 ? 
A1 O7 A1 16.9(3) . 5_655 ? 
T1 O7 A2 123.6(6) 6 7 ? 
T1 O7 A2 95.5(6) . 7 ? 
A1 O7 A2 16.6(5) . 7 ? 
A1 O7 A2 16.5(5) 5_655 7 ? 
T1 O7 A2 95.5(6) 6 3_545 ? 
T1 O7 A2 123.6(6) . 3_545 ? 
A1 O7 A2 16.6(5) . 3_545 ? 
A1 O7 A2 16.5(5) 5_655 3_545 ? 
A2 O7 A2 28.6(12) 7 3_545 ? 
T1 O7 O5 36.46(3) 6 6 ? 
T1 O7 O5 158.22(10) . 6 ? 
A1 O7 O5 75.06(5) . 6 ? 
A1 O7 O5 71.61(5) 5_655 6 ? 
A2 O7 O5 87.2(6) 7 6 ? 
A2 O7 O5 59.2(6) 3_545 6 ? 
T1 O7 O5 158.22(10) 6 . ? 
T1 O7 O5 36.46(3) . . ? 
A1 O7 O5 75.06(5) . . ? 
A1 O7 O5 71.61(5) 5_655 . ? 
A2 O7 O5 59.2(6) 7 . ? 
A2 O7 O5 87.2(6) 3_545 . ? 
O5 O7 O5 138.98(8) 6 . ? 
T1 O7 O6 128.84(9) 6 . ? 
T1 O7 O6 35.26(4) . . ? 
A1 O7 O6 115.26(9) . . ? 
A1 O7 O6 122.75(7) 5_655 . ? 
A2 O7 O6 106.4(5) 7 . ? 
A2 O7 O6 131.9(5) 3_545 . ? 
O5 O7 O6 161.68(7) 6 . ? 
O5 O7 O6 59.18(4) . . ? 
T1 O7 O6 35.26(4) 6 6 ? 
T1 O7 O6 128.84(9) . 6 ? 
A1 O7 O6 115.26(9) . 6 ? 
A1 O7 O6 122.75(7) 5_655 6 ? 
A2 O7 O6 131.9(5) 7 6 ? 
A2 O7 O6 106.4(5) 3_545 6 ? 
O5 O7 O6 59.18(4) 6 6 ? 
O5 O7 O6 161.68(7) . 6 ? 
O6 O7 O6 102.58(8) . 6 ? 
T1 O7 O1 34.67(4) 6 6 ? 
T1 O7 O1 103.03(7) . 6 ? 
A1 O7 O1 131.16(11) . 6 ? 
A1 O7 O1 119.08(13) 5_655 6 ? 
A2 O7 O1 134.4(3) 7 6 ? 
A2 O7 O1 114.8(5) 3_545 6 ? 
O5 O7 O1 61.42(3) 6 6 ? 
O5 O7 O1 125.63(6) . 6 ? 
O6 O7 O1 112.82(6) . 6 ? 
O6 O7 O1 60.26(4) 6 6 ? 
T1 O7 O1 103.03(7) 6 . ? 
T1 O7 O1 34.67(4) . . ? 
A1 O7 O1 131.16(11) . . ? 
A1 O7 O1 119.08(13) 5_655 . ? 
A2 O7 O1 114.8(4) 7 . ? 
A2 O7 O1 134.4(3) 3_545 . ? 
O5 O7 O1 125.63(6) 6 . ? 
O5 O7 O1 61.42(3) . . ? 
O6 O7 O1 60.26(4) . . ? 
O6 O7 O1 112.82(6) 6 . ? 
O1 O7 O1 68.99(5) 6 . ? 
T1 O7 O7 103.71(7) 6 5_656 ? 
T1 O7 O7 103.71(7) . 5_656 ? 
A1 O7 O7 70.91(16) . 5_656 ? 
A1 O7 O7 87.77(17) 5_655 5_656 ? 
A2 O7 O7 79.76(6) 7 5_656 ? 
A2 O7 O7 79.76(6) 3_545 5_656 ? 
O5 O7 O7 98.04(4) 6 5_656 ? 
O5 O7 O7 98.04(4) . 5_656 ? 
O6 O7 O7 72.99(5) . 5_656 ? 
O6 O7 O7 72.99(5) 6 5_656 ? 
O1 O7 O7 133.15(7) 6 5_656 ? 
O1 O7 O7 133.15(7) . 5_656 ? 
T1 O7 O3 82.80(7) 6 1_554 ? 
T1 O7 O3 82.80(7) . 1_554 ? 
A1 O7 O3 89.73(16) . 1_554 ? 
A1 O7 O3 72.87(16) 5_655 1_554 ? 
A2 O7 O3 81.48(6) 7 1_554 ? 
A2 O7 O3 81.48(6) 3_545 1_554 ? 
O5 O7 O3 76.20(5) 6 1_554 ? 
O5 O7 O3 76.20(5) . 1_554 ? 
O6 O7 O3 117.34(5) . 1_554 ? 
O6 O7 O3 117.34(5) 6 1_554 ? 
O1 O7 O3 60.47(4) 6 1_554 ? 
O1 O7 O3 60.47(4) . 1_554 ? 
O7 O7 O3 160.64(9) 5_656 1_554 ? 
T1 O7 M3 71.87(6) 6 . ? 
T1 O7 M3 71.87(6) . . ? 
A1 O7 M3 125.49(16) . . ? 
A1 O7 M3 108.63(16) 5_655 . ? 
A2 O7 M3 116.06(10) 7 . ? 
A2 O7 M3 116.06(10) 3_545 . ? 
O5 O7 M3 87.51(4) 6 . ? 
O5 O7 M3 87.51(4) . . ? 
O6 O7 M3 97.15(4) . . ? 
O6 O7 M3 97.15(4) 6 . ? 
O1 O7 M3 38.19(3) 6 . ? 
O1 O7 M3 38.19(3) . . ? 
O7 O7 M3 163.60(9) 5_656 . ? 
O3 O7 M3 35.76(3) 1_554 . ? 
T1 O7 A1 88.59(8) 6 5_656 ? 
T1 O7 A1 88.59(8) . 5_656 ? 
A1 O7 A1 113.25(14) . 5_656 ? 
A1 O7 A1 130.1(3) 5_655 5_656 ? 
A2 O7 A1 120.68(17) 7 5_656 ? 
A2 O7 A1 120.68(17) 3_545 5_656 ? 
O5 O7 A1 108.65(5) 6 5_656 ? 
O5 O7 A1 108.65(5) . 5_656 ? 
O6 O7 A1 53.95(5) . 5_656 ? 
O6 O7 A1 53.95(5) 6 5_656 ? 
O1 O7 A1 101.29(10) 6 5_656 ? 
O1 O7 A1 101.29(10) . 5_656 ? 
O7 O7 A1 42.34(12) 5_656 5_656 ? 
O3 O7 A1 157.02(12) 1_554 5_656 ? 
M3 O7 A1 121.26(12) . 5_656 ? 
T1 O7 O6 146.61(7) 6 2_656 ? 
T1 O7 O6 74.95(4) . 2_656 ? 
A1 O7 O6 51.59(10) . 2_656 ? 
A1 O7 O6 63.54(12) 5_655 2_656 ? 
A2 O7 O6 48.1(3) 7 2_656 ? 
A2 O7 O6 68.0(4) 3_545 2_656 ? 
O5 O7 O6 121.05(5) 6 2_656 ? 
O5 O7 O6 53.67(3) . 2_656 ? 
O6 O7 O6 64.45(4) . 2_656 ? 
O6 O7 O6 119.47(6) 6 2_656 ? 
O1 O7 O6 177.24(6) 6 2_656 ? 
O1 O7 O6 109.19(3) . 2_656 ? 
O7 O7 O6 46.48(3) 5_656 2_656 ? 
O3 O7 O6 120.71(5) 1_554 2_656 ? 
M3 O7 O6 141.17(3) . 2_656 ? 
A1 O7 O6 76.90(9) 5_656 2_656 ? 
T1 O7 O6 74.95(4) 6 5_656 ? 
T1 O7 O6 146.61(7) . 5_656 ? 
A1 O7 O6 51.59(10) . 5_656 ? 
A1 O7 O6 63.54(12) 5_655 5_656 ? 
A2 O7 O6 68.0(4) 7 5_656 ? 
A2 O7 O6 48.1(3) 3_545 5_656 ? 
O5 O7 O6 53.67(3) 6 5_656 ? 
O5 O7 O6 121.05(5) . 5_656 ? 
O6 O7 O6 119.47(6) . 5_656 ? 
O6 O7 O6 64.45(4) 6 5_656 ? 
O1 O7 O6 109.19(3) 6 5_656 ? 
O1 O7 O6 177.24(6) . 5_656 ? 
O7 O7 O6 46.48(3) 5_656 5_656 ? 
O3 O7 O6 120.71(5) 1_554 5_656 ? 
M3 O7 O6 141.17(3) . 5_656 ? 
A1 O7 O6 76.90(9) 5_656 5_656 ? 
O6 O7 O6 72.55(4) 2_656 5_656 ? 
T1 O7 O3 70.30(5) 6 . ? 
T1 O7 O3 70.30(5) . . ? 
A1 O7 O3 172.09(17) . . ? 
A1 O7 O3 171.05(17) 5_655 . ? 
A2 O7 O3 165.7(6) 7 . ? 
A2 O7 O3 165.7(6) 3_545 . ? 
O5 O7 O3 106.74(4) 6 . ? 
O5 O7 O3 106.74(4) . . ? 
O6 O7 O3 60.95(4) . . ? 
O6 O7 O3 60.95(4) 6 . ? 
O1 O7 O3 54.29(4) 6 . ? 
O1 O7 O3 54.29(4) . . ? 
O7 O7 O3 101.18(8) 5_656 . ? 
O3 O7 O3 98.18(5) 1_554 . ? 
M3 O7 O3 62.42(4) . . ? 
A1 O7 O3 58.84(12) 5_656 . ? 
O6 O7 O3 123.01(5) 2_656 . ? 
O6 O7 O3 123.01(5) 5_656 . ? 
 
_diffrn_measured_fraction_theta_max    0.950 
_diffrn_reflns_theta_full              40.71 
_diffrn_measured_fraction_theta_full   0.950 
_refine_diff_density_max    0.983 
_refine_diff_density_min   -1.366 
_refine_diff_density_rms    0.138 
